Upcoming SlideShare
×

# 1 etd

661 views

Published on

• Full Name
Comment goes here.

Are you sure you want to Yes No
• Be the first to comment

• Be the first to like this

### 1 etd

1. 1. PREDICTION OF LINEAR VISCOELASTIC RESPONSE OF THE LOSS SHEAR MODULUS OF POLYMER-MODIFIED BINDERS James W. Bryant, Jr. Thesis submitted to the faculty of Virginia Polytechnic Institute and State University in partial fulfillment of the requirements for Master’s Degree in Civil Engineering (Civil Infrastructure Engineering) Imad L. Al-Qadi, Chair Toni Triani Gerardo Flintsch March 19, 1999 Blacksburg, Virginia Keywords: polymer modified asphalt, shear modulus, viscoelasticity Copyright 1999, James William Bryant, Jr. i
2. 2. PREDICTION OF LINEAR VISCOELASTIC RESPONSE OF THE LOSS SHEAR MODULUS OF POLYMER-MODIFIED BINDERS by James W. Bryant, Jr. Abstract Current mathematical models, developed on straight asphalt binders, are inadequateto characterize the frequency dependence of response of polymer-modified asphaltbinders. In an earlier study at Virginia Tech, mathematical models were developed topredict the storage and loss shear moduli of polymer-modified binders. However themodel developed for the loss shear moduli is limited at high frequency (G” ≤ 107.5 Pa).This thesis presents a statistical modeling of loss shear modulus of polymer (randomcopolymers and thermoplastic block copolymers) modified binder. Data from dynamicmechanical analysis on modified binders, at temperatures between 5 and 75°C andfrequencies ranging from 0.06 to 0188.5 rad/s, were reduced to dynamic master curves ofmoduli, and used to develop the model. Twenty-one polymer-binder blends prepared andtested earlier at Virginia Tech where included in the study. Realistic characterization ofloss shear moduli values was obtained using the Gompertz statistical model. The modelwas validated by using mean square error of prediction (MSEP) in which a second set offrequency data was input in the model to obtain the moduli values, which were comparedto the measured data of the second set. Although this model was successfully tested forshear loss modulus prediction of polymer-modified binders, caution should be exercisedwhen it is applied, as such a model should be able to predict the storage modulus for aknown phase angle. ii
3. 3. Acknowledgments I thank GOD for leading me to Virginia Tech for graduate school. I am extremelygrateful to Dr. Al-Qadi, who gave me the opportunity to work on this project. I would liketo thank the other committee members, Dr. Triani and Dr. Flintsch , for their commentsand support. I would like to thank Fariborz Gahvari, a former graduate student, for the original workon which this research is built upon. Finally I would like to thank my family and my church for their support throughout thisprocess. iii
4. 4. TABLE OF CONTENTSChapter 1. Introduction......................................................................................................1 1.1 Background ...............................................................................................................1 1.2 Problem Statement ...................................................................................................3 1.3 Objectives..................................................................................................................3 1.4 Scope ........................................................................................................................4Chapter 2. Literature Review.............................................................................................6 2.1 Introduction ...............................................................................................................6 2.2 Asphalt Cement Types and Properties .....................................................................6 2.3 Binder Tests and Evaluation .....................................................................................8 2.3.1 Consistency Tests .............................................................................................9 2.3.2 SuperPaveTM Tests..........................................................................................11 2.4 Polymers .................................................................................................................13 2.4.1 Random Copolymers.......................................................................................14 2.4.2 Thermoplastic Block Copolymers....................................................................14 2.5 Polymerized Asphalt ...............................................................................................15 2.6 Linear Viscoelastic Theory......................................................................................16 2.6.1 Dynamic Response .........................................................................................17 2.7 Time-Temperature Superposition ...........................................................................20 2.8 Models Developed For Frequency Dependence of Asphalt Binder ......................23 2.8.1 Jongepier and Kuilman’s Model ......................................................................27 2.8.2 Dobson’s Model ...............................................................................................29 2.8.3 Dickenson and Witt’s Model ............................................................................31 2.8.4 Christensen and Anderson’s Model ................................................................32 2.8.5 Gahvari’s Model...............................................................................................34 2.8.6 Stastna’s Model ...............................................................................................37 2.8.7 Marasteanu and Anderson Model ...................................................................38Chapter 3. Research Program.........................................................................................39 3.1 Materials and Specimen Preparation......................................................................39 3.2 Data Collection and Analysis ..................................................................................42 3.3 Comparison of Recent and Previous Data Analysis...............................................43 iv
5. 5. Chapter 4. Model Development for Frequency Dependency of Loss Moduli ............49 4.1 Background .............................................................................................................49 4.2 Gompertz Model......................................................................................................51 4.3 Model Validation and Comparison..........................................................................57 4.3.1 Validation .........................................................................................................57 4.3.2 Model Comparison ..........................................................................................61 4.4 Model Limitations ....................................................................................................62Chapter 5. Summary, Findings, Conclusions, and Recommendations .....................66 5.1 Summary.................................................................................................................66 5.2 Findings...................................................................................................................66 5.3 Conclusions.............................................................................................................67 5.4 Recommendations ..................................................................................................67References ........................................................................................................................68Appendix A. Dynamic Moduli isothermal, master curve (with reference temperatureof 25°C), and shift factor, aT ............................................................................................76Appendix B. SAS Input file............................................................................................161Appendix C. SAS Output File........................................................................................166Appendix D. Comparison between measured dynamic loss modului and resultsfrom the Gompertz .........................................................................................................170Vita ...................................................................................................................................213 v
6. 6. LIST OF FIGURESFigure 2-1. Current morphological model for asphalt binder. 8Figure 2-2. Testing setup for DSR. 12Figure 2-3. Schematics of a typical dynamic mechanical analysis in shear mode. 20Figure 2-4. Graphical presentation of time-temperature superposition (data from Virginia Tech 1994 experiment, with reference temperature 25°C). 24Figure 3-1. Dynamic storage modulus versus frequency at eight test temperatures for ARG3. 45Figure 3-2. Dynamic loss modulus versus frequency at eight test temperatures for ARG3. 46Figure 3-3. Dynamic storage modulus and loss modulus master curves for ARG3 (reference temperature 25°C). 47Figure 3-4. Loss tangent master curve for ARG3 (reference temperature 25°C). 48Figure 4-1. Comparison between measured dynamic loss modulus for ARC4 and results obtained from the logistic model. 50Figure 4-2. A graphical representation of proposed model for loss modulus. 52Figure 4-3. Effect of β on the location of Gompertz distribution model for 56 ARC3.Figure 4-4. Comparison between measured dynamic loss modulus for AUD3 and results obtained from the Gompertz Growth model. 60Figure 4-5. Comparison between measured dynamic loss modulus for AUD3 and results obtained from the hyperbolic model. 64Figure 4-6. Hyperbolic and Gompertz distribution models with an extended frequency range. 65 vi
7. 7. LIST OF TABLESTable 2-1. Table 2-1. Elemental Analyses of Representative Petroleum 7 Binders.Table 3-1. AC-20 Properties. 40Table 3-2. Typical properties of the random modifiers 40Table 3-3. Table 1-3. Typical properties of the thermoplastic block copolymer modifiers at 23oC. 41Table 4-1. Estimated parameters for the current proposed loss modulus model based on Least Squares Analysis (Gompertz Growth Model). 54Table 4-2. Estimated parameters for the hyperbolic model proposed by Gahvari (1995) for loss modulus based on Least Squares Analysis. 58Table 4-3. Evaluation of Mean Squared Error Prediction for both current and previous proposed models for loss modulus. 63 vii
8. 8. Chapter 1. Introduction1.1 Background The ability of our nation’s infrastructure to provide necessities such as shelter,transportation, water and waste disposal, is vital to our quality of life. Highways play amajor role in our infrastructure system. Over 94% of the surfaced roads in the UnitedStates are covered with flexible pavement (FHWA, 1990), hot-mix asphalt(HMA). Part ofthe flexible pavement highways fail prematurely due to increases in traffic, axle load andhigher tire pressure. The volume of truck traffic doubled from 1974 to 1989 (Nahas, et al.,1989). It is estimated that nearly 50% of all funds spent in the transportation area godirectly to construction, maintenance and rehabilitation of pavements (Lytton, 1991). Hot-mix asphalt (HMA) is composed of both mineral aggregate and asphalt binder.Although its performance is a function of both materials, the binder controls specificfailure modes, including fatigue cracking and low temperature cracking. The performanceof the binder, which is a viscoelastic material, is highly influenced by temperature and rateof loading (Lewandowski, 1994). There are three main types of distress that flexible pavement surfaces undergo: (1)high temperature permanent deformation; (2) load-associated fatigue cracking; and (3)low temperature cracking. The binder properties play a significant role in each type ofdistress. Types of permanent deformation include rutting, distortion, and shoving. Theprogressive movement of HMA materials under repeated loads causes rutting. It usuallyoccurs along the wheel path in the traffic direction. An asphalt binder that has a lowviscosity at intermediate to high temperatures is more likely to rut because of its inabilityto respond elastically to the applied stresses. Fatigue (or alligator) cracking is caused bycyclic stress on a pavement over an extended period of time. Stiff binder and/or low 1
9. 9. binder content also cause this type of distress. Low temperature cracking occurs whenthe binder becomes too brittle and it looses the ability to deform elastically. The behavior of asphalt binder is complicated, because it is a viscoelastic material.At intermediate to high temperatures, asphalt behaves like a viscous fluid, while at lowtemperatures, it acts like a brittle elastic solid. A new and more complex material isformed when polymeric modifiers are added to asphalt binder. In an effort to improve flexible pavement durability, different types of asphalt additiveshave been investigated. Modifications of asphalt binders using various types of polymericmaterials have been promoted as an attractive technique to improve binder propertiesand the overall performance of flexible pavements (Lewandowski, 1994; Bonemazzi etal., 1996; Fleckenstein et al., 1992). One researcher suggests that there are at least 22 benefits attributed to the additionof polymers to asphalt binder (Lewandowski, 1994). It has been suggested that the useof polymer additives in HMA reduces rutting and fatigue cracking, while maintaining anacceptable binder viscosity at medium to high service temperatures (Bonemazzi et al.,1996). In addition to being less susceptible to low temperature cracking, polymermodified asphalts are also more resistant to freeze thaw damage (Fleckenstein et al.,1992). There is no consensus among researchers on the effectiveness of polymermodification on the performance of asphalt binder. A number of investigators agree thatsignificant improvement in the resistance to permanent deformation is obtained whenpolymer modified binders are used in flexible pavements (Fleckenstein et al., 1992;Srivastave et al., 1992; Little, 1992; Collins et al., 1992; Ponniah et al., 1996; Maccarroneet al., 1997). Polymer modifiers have also been found to increase the fatigue life offlexible pavements (Maccarrone et al., 1997). However, there is discussion on theeffectiveness of polymer additives as it pertains to improved low temperature properties.Some researchers find polymeric modification of asphalt binder beneficial (King et al., 2
10. 10. 1993; Stock et al.1992), while others state its effect to be negligible (Anderson et al.,1992; Bonemazzi et al., 1996; Gahvari 1995; Freeman et al., 1997).1.2 Problem Statement Characterizing the viscoelastic behavior of asphalt binder requires obtaining theresponse of the material over a wide range of temperatures and frequencies (i.e., loadingtime). Several researchers have produced models that mathematically describe thetemperature and the time dependency of straight asphalt binders (Jongepier andKuilman, 1969; Dobson, 1969; Dickinson and Witt, 1974; Christensen and Anderson,1992; Stastna et al., 1996). These models were not developed for predicting theviscoelastic response of modified binders; consequently, they have been found toproduce considerable discrepancies with experimental data (Gahvari, 1995). Fewresearchers have proposed mathematical describing the response of polymer-modifiedbinder (Gahvari, 1995; Stastna et al., 1996, Marasteanu and Anderson, 1999). The model presented by Gahvari is the most practical model proposed to date.However, there are certain limitations inherent in each model. The proposed model forstorage modulus is valid only for moduli below 108 Pa; above this value, the moduli tendto be overestimated. The proposed loss modulus model is symmetrical in shape withrespect to the peak point and therefore must be restricted to a specified range (Gahvari,1995).1.3 Objectives The objective of this study was to develop a model to describe the frequencydependence of the response of polymer modified binders, over the entire range oftemperatures and frequencies. The developed model was compared to the datacollected from previous experiments at conducted Virginia Tech. 3
11. 11. 1.4 Scope Characterization of the linear viscoelastic response of the polymer-modified binder isgenerally made possible by interpretation of dynamic master curves. At Virginia Tech,experimental research was conducted to characterize the complex moduli of polymermodified asphalt binders using a Dynamic Shear Rheomoter. Dynamic mechanicalanalysis was conducted on 21 binder-polymer blends at frequencies between 0.06 to188.5 rad/s and temperatures ranging from 5° to 75°C. The mixes were prepared usingone viscosity graded binder and seven different polymer modifiers. Each polymericadditive was blended with asphalt binder at three different concentration levels. Themodifiers were thermoplastic block copolymers and random copolymers, which arecommonly used in industry. The polymers selected represented a wide range of chemicalstructures and mechanical and physical properties. The study also investigated theeffect of short term aging on rheological properties of the modified blends. The linear viscoelastic range of response was established by performing stresssweeps over the entire range of temperatures at the desired frequencies. Isothermalgraphs of dynamic moduli data verses frequency were obtained as a result of frequencysweeps. Master curves were developed for the dynamic moduli over several decades ofreduced frequency by the application of time-temperature superposition. These mastercurves were used in order to characterize the response of the material. Twomathematical models were proposed to discuss the frequency dependence of theresponse and presented in earlier studies (Gahvari, 1995; Gahvari and Al-Qadi, 1996). Using the collected isothermal data, time superposition has been employed toreconstruct the dynamic master curves of all 21 polymer-binder blends (using sevenpolymers, each at three levels of concentration). The shifted moduli data was used toderive model constants by use of nonlinear regression analysis. Statistical analysis was performed comparing experimental data against datagenerated by the suggested model to determine its’ level of accuracy. In addition, the 4
12. 12. model accuracy was compared to that of the previous model developed during theoriginal Virginia Tech Experiment. This thesis contains Five chapters. Chapter 2 is an overview of binder types,rheological properties, polymeric modifiers, linear viscoelastic theory, time-temperaturesuperposition, and current research on the modeling of straight and modified binders.Chapter 3 presents the research program including the materials and specimenpreparation, data collection and previous analyses. Chapter 4 describes the modeldevelopment, where a new statistical model is introduced to describe the frequencydependency of the loss shear modulus and the evaluation and validation of the suggestedmodel. Chapter 5 presents the summary, findings and conclusions, as well asrecommendations for future research. 5
13. 13. Chapter 2. Literature Review2.1 Introduction Asphalt binder is one of the oldest engineering materials used by man. Thewaterproofing and adhesive qualities of asphalt make it suitable for use as roofing andpaving materials. The first use of asphalt as a paving material occurred during the1800’s. Hot-mix asphalt (HMA) is a composite mixture consisting of a number ofinterfaces and phases, and is used to construct flexible pavements. Asphalt binder is aviscoelastic material; therefore, at high temperatures it behaves like a viscous fluid and atlow temperature it behaves like an elastic solid. Therefore, behavior of HMA is highlydependent on the binder properties as temperature and rate of loading are varied. Modifiers, such as polymers, are added to asphalt binder to enhance its properties.The result of this modification increases the complexity of the material structure. Sincethe binder plays such an important role in the behavior of HMA, it is imperative tounderstand the behavior of asphalt binder, its components and their interaction. Thischapter provides an overview of the nature of asphalt binder, the tests used tocharacterize it, types of polymers used in asphalt binder, asphalt-polymer interaction,linear viscoelastic theory, and current research on straight and polymer-modified bindercharacterization.2.2 Asphalt Cement Types and Properties The composition of asphalt binder is very diverse. It is composed of nonpolarsaturated hydrocarbons and polar aromatic molecules (heteroatoms). Small amounts ofheavy metals are also found in asphalt binder (Table 2-1) 6
14. 14. Table 2-1. Elemental Analyses of Representative Petroleum Binders (After Roberts, et al., 1996). Composition (%) Element Mexican Arkansas-Louisiana Boscan California Carbon 83.77 85.78 82.90 86.77 Hydrogen 9.91 10.19 10.45 10.93 Nitrogen 0.28 0.26 0.78 1.10 Sulfur 5.25 3.41 5.43 0.99 Oxygen 0.77 0.36 0.29 0.20 Vanadium (ppm) 180 7 1380 4 Nickel (ppm) 22 0.4 109 6 The chemical composition and binder morphology influence the rheological propertiesof asphalt binder, which in turn affects the pavement performance. The current asphaltmorphological model divides the many different asphalt molecules into two classes: polarand non-polar. The polar molecules associate through hydrogen bonding, forming aweak network within the non-polar medium. The weak network of hydrogen bondsdissociate under increased heat or loading. The non-polar molecules act as the matrix forthe polar network and predominately affect the low temperature stiffness (Mckay et al.,1995). Three integrated phases or fractions are used in order to characterize asphalt: (1)asphaltenes; (2) resins; and (3) oils. Asphaltenes, the primary component of asphalt, aremulti-ring, polar, aromatic compounds that give asphalt its structure. They aresurrounded by moderately polar aromatic molecules and dispersed in the continuous non- 7
15. 15. polar oily phase. Resins are intermediate molecular weight materials that contain moreside chains than asphaltenes. They are semi-solid fractions that act as peptizing agents,which keep the asphaltene molecules from coagulation (Kerbs and Walker, 1971). Oilsyield asphaltene and resin molecules upon oxidation. They are soluble in most solventsand have both paraffinic and naphthenic structures. (a): High temperature (b) Low Asphalttene Maltene liquid Figure 2-1. Current morphological model for asphalt binder. The physical properties of asphalt binder are a function of the relative proportion of theintegrated fractions: asphaltenes, resins and oils. Newtonian behavior is generallyexhibited by binders containing a high degree of peptized asphaltenes, while binders withlow dispersed asphaltenes exhibit non-Newtonian flow. Figure 2-1 depicts the currentmorphological model used for asphalt binder. Other morphological models exist butFigure 2-1 is the most widely accepted.2.3 Binder Tests and Evaluation Traditionally, a variety of test methods have been used to characterize theconsistency, aging, and physical properties of asphalt binder. The penetration andviscosity tests are used to characterize temperature susceptibility. Asphalt binderspecifications were developed around these physical tests. These tests are empirical in 8
16. 16. nature, which place certain limitations on the results that they provide. Pavementperformance experience is required before the test results yield meaningful information.The relationships between the test results and the performance may not be accuratebecause the tests do not take into account the mechanistic properties i.e. stresses andstrains. In recent years, it became apparent that new test methods were needed, both for usein specifications and in developing correlation between physical and chemical propertiesfor binder characterization. Fundamental material properties expressed in engineeringunits are needed in order to accurately develop relationships between the properties ofasphalt binder and HMA. These fundamentally sound relationships are used to developmodels that relate binder properties to mixture properties and finally to pavementperformance. The Strategic Highway Research Program (SHRP) proposed a newsystem for binder specification. These new binder specification tests are performancebased, expected to be better correlated to field results, and take into account bothrheological and mechanistic failure modes. The following section summarizes theconventional consistency tests for asphalt binder and Superpave Binder Specificationtests.2.3.1 Consistency Tests Consistency describes the degree of fluidity of asphalt binder at any given testtemperature. Since asphalt binder is a viscoelastic material, its consistency varies withtemperature. It is essential to measure the consistency of different binders at the sametemperature and loading rate if comparisons between binders are to be made. Penetration Test The penetration test is an empirical measure of the consistency of an asphalt binderand is measured in accordance with ASTM D 5 (Annual Book of ASTM Standards, 1996).The test is performed by measuring how far a stainless steel needle penetrates aspecimen of asphalt binder when loaded with 100 g for 5 s at a temperature of 25°C 9
17. 17. (77°F) (Annual Book of ASTM Standards, 1996). The farther the needle penetrates the“softer” the binder. For binders used in the United States, the typical penetration numberrange is 60-100, which represents a penetration range of 15- 25 mm (0.6 – 1 in). Viscosity Tests Absolute viscosity is measured in accordance with ASTM D 2171 (Annual Book ofASTM Standards, 1996) using a U-shaped capillary tube viscometer. An asphalt bindersample is heated to temperature of 60°C and is poured into the viscometer. Under theaction of a vacuum the binder rises (flows) and passes through timing marks. Themeasured time of flow between two successive timing marks on the capillary tube ismultiplied by the calibration factor (provided by the manufacturer) of the viscometer. Theresult of this test yields the viscosity of the binder in units of poise. Paving grade asphaltsare classified into six groups based on the viscosity grading system: AC-2.5, AC-5, AC-10, AC-20, AC-30 and AC-40. The digital number represents the viscosity of the binder in100 poise. The kinematic viscosity is performed at 135°C. It is measured in accordance withASTM D 2170 (Annual Book of ASTM Standards, 1996) using a cross-armed viscometer.Here the binder flows under the force of gravity rather than vacuum application. Theprocedure is similar to the absolute viscosity test and results are usually defined in unitsof centistokes. These tests do not provide information about binder properties over the entire range oftypical in-place pavement temperatures. The standard test temperatures of 60°C and135°C may provide information about the higher temperature viscous behavior. However,the binder behavior at low temperatures cannot be realistically determined from dataobtained from the viscosity tests. 10
18. 18. 2.3.2 SuperPaveTM Tests Rotational Viscometer This test method is used in order to determine the viscosity of asphalt binder at hightemperatures, usually above 100°C. This information is needed to determine thepumping and mixing temperatures. This test method is performed in accordance toAASHTO TP 48. The rotational viscosity is determined by measuring the torque requiredto maintain a constant rotational speed (20 RPM) of a special spindle in an asphalt bindersample at a constant temperature. The SuperPaveTM binder specifications limit theviscosity to 3 Pa⋅s at 135°C. Dynamic Shear Rheometer (DSR) The Dynamic Shear Rheometer (DSR) is used to measure rheological properties,such as the linear viscoelastic moduli of binders at intermediate to upper servicetemperatures. The DSR is used for specification purposes to measure the complexmodulus and the phase angle of asphalt binders at a frequency of 10 rad/s, where thecomplex modulus is approximately 10 Mpa or greater. The DSR can be used todetermine the time (frequency) dependency of the modulus. In order to constructthermorheologically simple linear viscoelastic master curves, time-temperaturesuperposition can be applied to data obtained from the DSR. Figure 2-2 illustrates the testing setup for the DSR. In general, the asphalt bindersample is placed between two plates; the bottom plate being fixed, while the upper plateoscillates. The centerline of the plate, point A, moves to point B as the plate oscillates.The centerline then passes through point A and moves to point C, after which thecenterline returns to point A. This test is performed on both aged and unaged binderspecimen. 11
19. 19. Position of Oscillating Plate Applied Stress or Strain B Asphalt Oscillating A Plate A A C B C A Fixed Plate 1 Cycle Figure 2-2. Testing setup for DSR. Bending Beam Rheometer (BBR) The Bending Beam Rheometer (BBR) test the properties of asphalt binders at lowservice temperatures (below 5°C) to determine its’ susceptibility to thermal cracking. Thetesting procedure is given by AASHTO TP1. The BBR measures stiffness using atransient creep load, applied in bending mode, to load a beam specimen constructed withasphalt binder held at a constant low temperature. Rolling Thin Film Oven (RTFO) The Rolling Thin Film Oven (RTFO) test simulates the short term aging of asphaltbinder, which usually takes place in the mixing plant and during hauling and constructionof HMA. This test is performed in accordance to ASTM D2872 (Annual Book of ASTMStandards, 1996). A certain amount of asphalt is poured into a bottle and placed on arotating rack inside an oven maintaining a temperature of 163°C. The rack rotates whilea hot air jet with a specified discharge is blown into the sample. This test takesapproximately 75 to 85 minutes. 12
20. 20. Pressure Aging Vessel (PAV) The Pressure Aging Vessel (PAV) test exposes the binder to high pressure andtemperatures to simulate the effects of long term aging. The pressure vessel is designedto operate under a pressure of 2070 kPa and temperature conditions ranging from 90° –110°C. The sample rack is placed in a preheated unpressurized PAV. When the vesseltemperature is within 2°C of the desired temperature, the pressure is applied and thetiming for the aging process begins. After 20 hours, the pressure is gradually removed.This test is performed on binder that has been aged using the RTFO method.2.4 Polymers Polymers are large molecules constructed from a number of smaller structural unitscalled monomers. These monomers are covalently bonded in any conceivable pattern.Monomers have two or more bonding sites, through which they can be linked to anothermonomers to form a polymer chain. Homopolymers (or simply polymers) occur whenonly one species of monomer is used to construct a macromolecule. If themacromolecule consists of two types of monomer units, it is referred to as a copolymer. Polymers can be grouped into three major categories: plastics, fibres and elastomers.There is no defining line that separates polymer groups. One method of defining amember of these categories is to observe the load-deformation behavior. Fibres and rigidplastics are resistant to deformation and are characterized by a high modulus and lowpercentage elongation. Elastomers exhibit behavior similar to that of a rubber band, i.e.,increasing tensile strength with increased elongation and the ability to recover to the initialstate after removal of the load (King and King, 1986). As it pertains to asphalt binders, the major elastomeric modifiers include styrene-butadiene-styrene (SBS), styrene-isoprene-styrene (SIS), styrene-ethylene/butadiene-styrene (SEBS), and styrene-butadiene rubber. The plastomeric modifiers are ethylene-vinyl-acetate (EVA), polyvinylchloride (PVC), and polyethylene/polypropylene. As 13
21. 21. compared to plastomeric modifiers, elastomeric modifiers are more commonly used in themodification of asphalt binder. The thermoplastic elastomeric modifiers used in this study mainly consisted of randomcopolymers and block copolymers. The following section discusses their mechanicalproperties and molecular structure.2.4.1 Random Copolymers Random copolymers are synthesized by statistical placement of monomer units alonga polymer chain backbone (Nosky and McGrath, 1977). They are homogeneous systemsthat exhibit characteristics between the two extremes of the reacting monomers. Unlikeblock copolymers, random copolymers do not form polymer networks and have a single-phase morphology. Styrene-butadiene rubber (SBR) is an example of a randomcopolymer.2.4.2 Thermoplastic Block Copolymers Thermoplastic block copolymers are formed through the process of reactingmonomers together. The three general structures for block copolymers are tri-blocklinear, radial (or branched) systems and linear diblock structures. Tri-block linearstructures are denoted as A-B-A, where A is a thermoplastic end-block, such aspolystyrene and B is a rubbery mid-block, such as polybutadiene or polyisoprene.Styrene-butadiene-styrene (SBS) and styrene-isoprene-styrene (SIS) are examples of tri-block copolymers. Styrene-ethylene/butadiene-styrene and styrene-ethylene/propylene-styrene are formed by hydrogenation of the rubbery mid-block, therefore creating anotherversion of these copolymers. This structure represents a two-phase system in which therubbery mid-block forms a continuous phase of three-dimensional elastomeric networkcontaining the dispersed end-block phase (Holden et al., 1969). Radial (or branched)systems are of the (A-B)n type. Examples of this system include (SB)n and (SI)n. Diblocklinear structures are depicted by A-B; examples include SB, SEP, and SEB. 14
22. 22. Block copolymers can be synthesized in three ways: (1) ionic initiators, where anactive site is kept alive on the end of the initial block, which is then capable of initiatingchain growth of the second monomer on the end of the first chain; (2) coupling of differentblocks with functional terminal units, either directly or through a reaction involving a smallintermediate molecule; and (3) bifunctional radial initiators, where a second potentialactive site is incorporated at the one end of the first chain grown, which can initiate at alater stage a new chain from the macro-radial produced (Cowie, 1991). Inherent thermodynamic incompatibilities exist in thermoplastic copolymers betweenthe end block and the rubbery mid-block. End-blocks, such as polystyrene, act asphysical cross-links connected by rubbery springs forming a three dimensional rubberysystem at temperatures below Tg, the glass transition temperature. At temperaturesabove Tg, the cross-linked network becomes less rigid and softens in the presence ofshear. It is at this stage that polymers can be incorporated into asphalt. This process isreversed upon cooling therefore the rigid domains and the network reform and impartselasticity and tensile strength to the polymer-asphalt blend.2.5 Polymerized Asphalt For a polymer to be effective in HMA, it should blend with the binder and improve itsresistance to vehicular and environmental loading. There is a complex relationshipbetween the chemical composition and morphology of an asphalt binder and its physicaland rheological properties. Critical to the process of polymer modification of asphaltbinder is the compatibility of the system. In modifying asphalt binder with polymericmaterials, a change in its chemical composition and structure occurs, which in turn affectsits properties. The polymer modification or blending process of asphalt binder may resultin one of three type mixtures: (1) heterogeneous; (2) totally homogenous; and (3) micro-heterogeneous. A heterogeneous mixture is one in which phase separation occurs,meaning that the binder and polymer are incompatible. In a totally homogeneous mixturethe polymer is completely soluble in the oils of the binder, which inhibits anyintermolecular interactions. This creates a stable binder, while only slightly improving the 15
23. 23. binder properties. A micro-heterogeneous mixture is made up of two distinct finelyinterlocked phases. In this system, the polymer swells, absorbing some of thenonasphatlene fraction of the binder forming a network composed of both a polymer andbinder phase (Brule, 1997). In binders containing SBS and SEBS, a polymeric network is formed which leads tothe enhanced performance of the binder, especially at elevated temperatures. Themodulus has been found to be temperature independent at higher temperatures;consequently the material exhibits more elastic behavior at higher temperatures (Bouldinand Collins, 1992). Block copolymers have been shown to form a continuous network within asphaltbinder at polymer concentrations as low as five percent by weight. Polymer modificationreduces the effects of oxidative aging. This may be caused by molecules in the binder,that are chemically active and bound to oxidize, to undergo micro-structural interactionswith the modifier and prevent the molecules from picking up an oxygen molecule(Srivastave, et al., 1992).2.6 Linear Viscoelastic Theory The response of viscoelastic materials is intermediate between the behavior of anelastic solid and a viscous fluid. In an elastic material, the strain response to an arbitrarystress is not time dependent. When loaded in creep, this material deforms immediately toa constant strain. When the load is removed, the material instantaneously returns to itsinitial shape. Under the application of a load, viscous materials deform at a constant rate,continuing until the load is removed. Unlike elastic materials, there is no recovery ofdeformation, i.e. it does not return to its initial state. The behavior of viscoelastic materials is time dependent and includes both elastic andviscous components. When loaded, viscoelastic materials do undergo some immediatedeformation, which corresponds to the elastic component of response. This deformation 16
24. 24. is followed by a gradual time dependent deformation that can be divided into twocomponents, delayed elastic and viscous. When the load is removed, the delayed elasticdeformation is recovered. This recovery does not occur instantaneously as seen in apurely elastic response. As stated earlier, there is no recovery of this deformation.2.6.1 Dynamic Response Dynamic mechanical analysis is one of the best tools used to characterize viscoelasticmaterial. These tests are performed in either stress or strain controlled modes. In thestress controlled mode, a sinusoidal stress is applied to the sample and the resultingstrain is monitored as a function of frequency. In the strain controlled mode, a sinusoidalstrain is applied and the stress is monitored with respect to time. Considering the strain controlled mode, the applied strain is defined as the real part ofa complex strain, ε* = ε\$ eiωt = ε\$ (cos ωt + i sin ωt) (2.1) ε(t) = ε\$ cos ωt (2.2)where, ε* = complex strain, ε(t) = applied strain, ε\$ = applied strain amplitude, t = time, s, and ω = frequency, rad/sThe stress output can also be considered as the real part of a complex stress: 17
25. 25. σ* = σ ei(ωt +δ) = σ [cos(ωt + δ) + i sin(ωt + δ)] \$ \$ (2.3) σ(t) = σ cos(ωt + δ) \$ (2.4)where, σ* = complex stress, σ(t) = stress output, Pa, σ = stress output amplitude, Pa, ˆ δ = phase angle, rad.In an elastic material, the applied strain and resulting stress are always in phase,therefore, δ = 0 rad. In a viscous material, the strain lags behind stress by π/2 rad (δ =π/2 rad). For a viscoelastic material the phase angle, δ, is always between 0 and π/2.The dynamic complex modulus can be defined as the ratio of complex stress to complexstrain: σ iδ \$ E* (iω) = σ*/ε* = e (2.5) ε\$The dynamic complex modulus can be resolved into two components: E* (iω)= E’ (ω)+ iE”(ω) (2.6)where, E’ (ω) = dynamic storage modulus, Pa, E”(ω)= dynamic loss modulus, Pa. 18
26. 26. The “in phase” and “out of phase” components of the complex modulus are representedby E’ (ω) and E”(ω), respectively. Furthermore, the absolute value of the complexmodulus can be computed as σ\$ E* (iω)= [ E ′(ω )] + [ E ′′(ω )] 2 2 = ε\$ (2.7)Through simple mathematical manipulation the following relationships exist: E’ = E*cos δ (2.8) E” = E*sin δ (2.9) tan δ = E’’/E’ (2.10)where tan δ is called the loss tangent and is a measure of relative energy dissipation. In shear mode, dynamic mechanical analysis yield moduli values represented by G*,G’ and G’’, which correspond to complex, storage and loss dynamic shear moduli. Figure2-3 shows the schematic of a typical dynamic mechanical analysis along with the relatedequations. Figure 2-3 shows, that at high frequencies (short loading times) the storage modulusis the major contributing component to the complex modulus. At low frequencies(corresponding to high temperatures), the complex modulus is approximately equal to theloss modulus ( |G*| ≅ G’’). Here it is observed that the slope of the complex modulus curveapproaches unity and viscous behavior is exhibited by the binder. 19
27. 27. γ\$ S T R A IN IN P U T : γ ( t ) = γ\$ c o s ω t δ τ\$ STRESS RESPONSE : τ ( t ) = τ\$ c o s(ω t + δ ) τ\$ G * = γ\$ COMPLEX MODULUS :Figure 2-3. Schematics of a typical dynamic mechanical analysis in shear mode. Dynamic mechanical analysis provides insight into the behavior of viscoelasticmaterials. The elastic and viscous components of response reflect the material’sbehavioral variations. These variations are due to changes in the material’smicrostructure, temperature or frequency. Dynamic moduli master curves areconstructed in order to view the response of the material over a broad range offrequencies or temperatures. The construction of these curves is contingent upon theapplicability of the principle of time-temperature superposition. The next sectiondescribes time-temperature superposition, as it pertains to the construction of mastercurves.2.7 Time-Temperature Superposition The modulus of a viscoelastic material is both time (frequency) and temperaturedependent. In viscoelastic experiments, moduli can be measured as a function oftemperature with constant time (frequency). The complete modulus-temperaturebehavior extends over several decades of frequency. It is not practical to perform 20
28. 28. dynamic mechanical test over wide ranges of frequency. Through time-temperaturesuperposition the frequency scale can be extended to encompass the entire modulus-temperature behavior for a viscoelastic measurement performed over a limited frequencyrange. Leaderman (1943) observed that the viscoelastic response curves, for a wide varietyof amorphous polymers obtained at different temperatures, were identical in shape anddiffered only in their location along the frequency (time) axis. Tobolosky and Eyring(1943) made similar observations leading to the introduction of the time-temperaturesuperposition principle (Andrews et al., 1948; Tobolosky, 1956). According to thisprinciple, viscoelastic data at any temperature can be translated to another temperatureby a simple multiplicative transformation of the time scale or an additive factor to the logtime-scale. Time-temperature superposition is applicable to thermorheologically simple materials(Schwarzl and Staverman, 1952). Thermorheologically simple materials are a specialclass of viscoelastic materials whose temperature dependence of mechanical propertiesis particularly responsive to analytical description (Haddad, 1995). These materials,which include a number of non-crystalline homopolymers and homogeneous copolymers,generally make up the simplest and most realistic viscoelastic constitutive equation forwhich response under constant temperature is used to predict the response undertransient temperatures. Although asphalt binder is complex in nature, it has been foundto exhibit the behavior of a thermorheologically simple material (Brodnyan et al., 1960;Wada and Hirose, 1960; Dickenson and Witt, 1974). In a thermorheologically simple material, a change in temperature results in a changein the rate of molecular motion. The sequence of molecular events is unchanged. Therate of molecular motion, as well as the sequence of molecular processes, is affected bychanges in temperature for a thermorheologically complex material. Forthermorheologically simple materials the relaxation times are assumed to be equally 21
29. 29. effected by changes in temperature (Schwarzl and Stavemen, 1952). This assumption isthe underlying principle behind time-temperature superposition. In thermorheologically complex materials the mechanical response curves cannot besuperimposed to form a master curve by a simple transition along the frequency axis.The shift factor for this class of material is a function of both temperature and frequency(Fesko and Tschoegl, 1971). Superposition may be applied to these types of materialsbut only by a point by point basis.Mathematically time-temperature superposition principle may be expressed as follows(Aklonis and MacKnight, 1983): F(T1, ω) = F(T2, ω/aT) (2.11)where, F(T1, ω) = value of a viscoelastic function at temperature T1 and frequency ω, F(T2, ω/aT) = value of viscoelastic function at temperature T2 and frequency ω/aT, aT = horizontal shift factor (which is a function of T1 and T2. In order to apply time-temperature superposition, dynamic mechanical tests must beperformed at several temperatures over a limited frequency range. The entire range ofdata, for a viscoelastic function (compliance, modulus, or loss tangent) is then plottedagainst frequency. A reference temperature is selected and the remaining curves areshifted along the frequency axis, partially overlapping, forming a continuous smoothmaster curve. The master curve extends over a wide range of frequencies. The amountto shift for each isothermal set of data is a measure of the temperature dependency ofresponse. Figure 2-4 presents a graphical illustration of time-temperature superposition. Three conditions must exist for time-temperature superposition to be applicable(Ferry, 1980). The response curves should have the same shape; shift factors for all 22
30. 30. viscoelastic functions should be unique; and the variations of shift factors withtemperature should follow a rational pattern.2.8 Models Developed For Frequency Dependence of Asphalt Binder The use of asphalt-polymer blends has been documented as early as 1902, when aFrench rubberized asphalt company laid rubberized asphalt roads (Thompson, 1979). Inthe 1930’s, a number of rubberized asphalt test roads were constructed by both theBritish and French (Lewandowski, 1994). In recent years, there has been an increased interest in the use of polymer modifiersin flexible pavements. During the past three decades there have been a number ofstudies investigating the cost effectiveness, application, behavior and the performance ofpolymer-modified asphalt binders. Several studies have addressed the performance ofpolymer modified binders and mixes under field conditions (Al Dhalaan, et al., 1992;Collins et al., 1992; Fleckenstein et al., 1992; Little, 1992; Maccarrone et al., 1997; Oliveret al., 1997; Ponniah et al., 1996; Seerfass et al., 1992; Stock and Arand 1992; Tayebaliet al., 1992; Thomas et al., 1996; Zhou et al.; 1994). Research has also been done in thearea of polymer-asphalt compatibility, microstructure, and polymer-asphalt interaction(Collins et al., 1991; King and King, 1986; Shuler et al., 1987). Other studies haveconcentrated on the effect of aging on the temperature susceptibility and rheologicalbehavior of modified binders (Anderson et al., 1992; Bonemazzi et al., 1996; Collins andBouldin, 1992; Gahvari, 1995; Gahvari and Al-Qadi, 1996; Huang et al., 1996; Oliver etal., 1997; Srivastava et al., 1992).Many of the aforementioned studies used dynamic mechanical analysis in thecharacterization of polymer-modified binders. Characterizing the viscoelastic behavior ofasphalt binder requires obtaining the response of the material over a wide range oftemperatures and frequencies (loading time). 23
31. 31. 1.0E+09 5°C 15°C 25°C 35°C Loss Modulus, (Pa) 1.0E+06 45°C 55°C 65°C 75°C 1.0E+03 log aT 1.0E+03 1.0E-01 1.0E-05 5 25 45 65 Temperature (°C) 1.0E+00 1.0E-02 1.0E+00 1.0E+02 1.0E-06 1.0E-03 1.0E+00 1.0E+03 Reduced Frequency (rad/s)Figure 2-4. Graphical presentation of time-temperature superposition (data from Virginia Tech 1994 experiment, with reference temperature 25°C). 24
32. 32. Several researchers have produced models that mathematically describe the temperatureand the time dependency of straight asphalt binders (Jongepier and Kuilman, 1969;Dobson, 1969; Dickinson and Witt, 1974; Christensen and Anderson, 1992). Thesemodels are not adequate in predicting the linear viscoelastic response of polymermodified binders. Until recently, no effort had been made to reduce the dynamicmechanical data on a wide variety of modified binders into the framework of mathematicalmodels. Anderson et al. (1992) studied rheological properties of asphalt emulsions modifiedwith SBS, SBR, and neoprene. Master curves were constructed from dynamicmechanical tests performed at temperatures ranging from –35 to 60 ° C. Andersonconcluded that the addition of polymer extends the relaxation process to longer times. Inorder to form smooth continuous curves of viscoelastic functions, both horizontal andvertical shift factors were used. The significance of the vertical shift factors is not certain.Moreover, no quantitative measure of shift in the relaxation spectra was established. TheWilliams Landel Ferry (WLF) equation (Williams et al., 1955) and the Arrhenius functionwas used in order to describe the temperature dependency above and below the Tg,respectively. Stock and Arrand (1993) investigated the rheological properties of six differentpolymer modified binders. Plastomeric and elastomeric modifiers were used in theirstudy. Dynamic mechanical tests were performed on the modified binders over a limitedrange of frequencies (0.1 to 10 Hz) and temperatures (40 to –10 ° C). The modelproposed by Dobson (1969) was used to describe the frequency dependency of theresponse. As stated earlier, there has been very little effort to reduce the dynamic mechanicaldata on a wide range of modified binders into the framework of mathematical models.Two researchers have produced models that can, with some degree of accuracy, predictthe dynamic response of polymer modified binders (Gahvari, 1995, Stastna et al., 1996,Marasteanu Anderson, 1999). 25
33. 33. Gahvari and Al-Qadi (1996) conducted dynamic mechanical analysis on 21 asphalt-polymer blends at frequencies between 0.06 to 188.5 rad/s temperatures ranging from 5°to 75° C. The mixes were prepared using one viscosity graded asphalt binder and sevendifferent polymer modifiers. Each polymeric additive was blended with asphalt binder atthree different concentration levels. The modifiers were thermoplastic block copolymersand random copolymers. The effect of short term aging on rheological properties of themodified blends was also investigated. Master curves were developed for the dynamicmoduli over several decades of reduced frequency. Two mathematical models, for G’and G” respectively, were proposed to discuss the frequency dependence of theresponse. The WLF equation was found to adequately describe the temperaturedependency of all modified binders used in that study. Stastna et al. (1996) performed dynamic mechanical analysis on five asphalt-polymerblends. The five modified binders were divided into two groups. Group 1 used a SBSmodifying agent and Group 2 contains binder that was modified with PE and EVA. A fractional model of complex modulus, based on the general principles for a linearresponse function, is used to depict the frequency dependency of the response. Themodel considers the polar form of G*, G* = |G*| exp (iδ). The values |G*| are slightlyunderestimated in the region of the Tg. Marasteneanu and Anderson (1999) proposed a modified version of the modeldeveloped by Christensen and Anderson. Testing was performed on 38 plain andmodified binders. As compared to the original Christensen and Anderson model, thedegree of precision was found to be greater. A brief description of previous models used to describe the dynamic response of bothmodified and unmodified binders is presented in the remaining part this section. 26
34. 34. 2.8.1 Jongepier and Kuilman’s Model Jongepier and Kuilman (1969) derived models for various rheological functions basedon the assumption that the relaxation spectra is approximately log normal in shape. Thismodel is expressed mathematically using a relatively complex set of mathematicalequations. The relaxation spectrum is given by:  ln τ / τ m  2 Gg H (τ ) = exp−   (2.12) β π  β where, β = width of the distribution function, τ = relaxation time, s, η −β 2 τm = time constant, s, defined by 0 e 4 , Gg η0 = Newtonian viscosity, Pa⋅s, Gg = Glassy modulus, Pa. The glassy modulus, Gg , is defined as the limiting value of storage modulus atextremely high frequencies and is expressed by: +∞ Gg = ∫ H (τ )d ln τ . (2.13) −∞In order to mathematically describe the loss and storage modulus, the followingtransformations were applied: 2 u = ln ωτ , and x = ln ω r (2.14) β2 27
35. 35. where, ωr is a dimensionless reduced frequency defined by ωη 0 ωr = (2.15) GgThe mathematical expressions for storage and loss moduli are given as:  β ( x − 1 / 2)  ∞  u  cosh( x + 1 / 2)u 2 2 Gg G ′( x ) = β π exp−   2  × ∫ exp−  β   0   cosh u du , (2.16)  β ( x − 1 / 2)  ∞  u  cosh( x − 1 / 2)u 2 2 Gg G ′′( x ) = β π exp−   2  × ∫ exp−  β   0   cosh u du , (2.17) Jongepier and Kuilman (1969) developed a set of master curves for complex modulusand phase angle for a wide variety of asphalt binders by integrating the above equations2.16 and 2.17 for a range of β values. The authors concluded that the variations in therelaxation spectra resulted from changes in the width parameter β. Comparisons weremade between experimental data and data generated by the model. It was discoveredthat the accuracy of the model for binders with small β was greater than that of binderswith large β values. It was reported that the response of binders with larger β values isless frequency dependent. The WLF equation (Williams et al., 1955) was used in order to describe thetemperature dependency of the response: 28
36. 36. C1 (T − TR ) log a T = − (2.18) C2 + (T − TR )where, a T = shift factor, TR = reference temperature, °K or °C, C1 and C2 = experimental constants. Jongepier and Kuilman stated that in order for the interpretation of constants C1 andC2 to be meaningful, TR should be selected to have a physical significance. However,through dylatometric glass transition temperature (Tg) measurements, they realized thatuse of Tg as the reference temperature does not result in a universal set of constants inthe WLF equation. The authors concluded that the glass transition temperature is not anappropriate parameter to describe the temperature dependence of asphalt cement.Defining TR as an equi-viscous temperature (a temperature at which asphalts have acertain viscosity), resulted in varying sets of C1 and C2 constants for different asphalttypes. Although this model is theoretically sound, it is not suitable for practical use, becauseof the mathematical complexity of the equations developed for frequency dependence.2.8.2 Dobson’s Model Dobson (1969) developed a model for frequency dependence of asphalt bindersbased on describing the complex modulus and loss tangent master curves as a functionof frequency. The proposed model by Dobson relating complex modulus and reducedfrequency is given by: 29
37. 37. 1 20.5 − Gr− b  − 1.02 log ωr = log Gr −  log(1 − Grb ) +  for Gr > 10 b , (2.19) b 230.3 where, η 0ωa T ωr = , (2.20) Gg G* Gr = , (2.21) Gg b = a parameter describing the width of relaxation spectrum. The other parameters were previously defined. Although b is defined as the widthparameter for relaxation spectrum, no further explanation has been made on it and it isnot clear what type of distribution function it refers to. The author states that b can belooked upon as a shear susceptibility parameter and is related to the penetration index. Dobson also used the WLF equation to describe the temperature dependency of theresponse of asphalt binders. He found that for T – TR > -20, the WLF, with universalconstants, can be used to fit the shift factor data. This agreed with the previous findingsby Brodnyan (1960). At lower temperatures, it was found that the WLF equationoverestimates the shift factors. Therefore, Dobson’s version of the WLF equationconsists of two pairs of constants for temperatures below and above the referencetemperature: −12.5(T − TR ) log a T = , T − TR < 0 , (2.22) 142.5 + (T − TR ) −8.86(T − TR ) log aT = , T − TR > 0 , (2.23) 1016 + (T − TR ) . 30
38. 38. Dobson did not specify a certain reference temperature, but like Jongepier and Kuilmanstated that TR should be an equi-viscous temperature for asphalts.2.8.3 Dickenson and Witt’s Model Dickinson and Witt (1974) developed analytical expressions for the complex modulusand phase angle in terms of frequency. These expressions were derived from dynamicmechanical data from 14 different asphalt binders. The master curves for complexmodulus and phase angle were treated mathematically as hyperbolas. The equationpresented for complex modulus is given by: log Gr = 1 2 [ ] log ω r − (log ω r ) 2 + (2 β ) , (2.24)Gr and ωr have been previously defined. This equation represents one arm of ahyperbola whose asymptotes, log Gr = log ωr and log Gr = 0. The values of theasymptotes indicate the viscous and elastic extremes of response, respectively. Theparameter β corresponds to shear susceptibility and is equal to the distance between theorigin of hyperbola and the master curve on the log Gr scale.The mathematical expression for phase angle is: π − 2δ ′  log ω r  δ = δ ′+ 1 − , (2.25) 4   (log ω r ) 2 + (2 β ) 2   31
39. 39. where, δ’ is a very small angle (less than 3°), which is assigned to the glassy modulus. Based on these two equations, Dickinson and Witt computed the values of storageand loss moduli and developed the relaxation spectra. They observed that the spectrawere not symmetrical with respect to the maximum value; concluding that the spectrawere not consistent with Jongepier and Kuilman’s assumption of log normal distributionfor relaxation times. Dickinson and Witt used the Dobson’s version of WLF equation to describe thetemperature dependency of their experimental data. Based on the two sets of constantsproposed by Dobson, they evaluated the reference temperature for the range of studiedasphalts.2.8.4 Christensen and Anderson’s Model Christensen and Anderson (1992) developed several master curves of complexmodulus and loss tangent for eight SHRP core asphalts. The frequency dependence ofthe response was describe by a mathematical model based on a modified logisticdistribution function for the resulting relaxation spectra. Complex modulus and phaseangle in terms of frequency were described by the following: R −  log 2  log 2  ωc  R  1 +   G (ω ) = G g * , (2.26)  ω    90 δ (ω ) = log 2 , (2.27) ω  R 1+   ωc  32
40. 40. where, ωc = crossover frequency, rad/s,  Gg  R = rheological index defined by log *   G (ω )  . (2.28)   ω =ω cThe remaining parameters are as previously defined. In this model, parameters ωc and Rhave considerable physical significance. The rheological index, R, is a shape parameterfor the master curve and represents the width of relaxation spectrum. Asphaltscharacterized by larger R values exhibit wider relaxation spectrum. The crossoverfrequency, ωc, represents the frequency at which δ = 45°. Several empirical observationshave confirmed that the crossover frequency usually coincides with the intersection ofglassy and viscous asymptotes of the complex modulus master curve. Therefore, it canbe regarded as a location parameter on the master curve. Through comparison between the experimental data and data generated by themodel, Christensen and Anderson observed some discrepancies for moduli belowapproximately 105 Pa. Moduli values below this range represent higher temperatures orloading times. Therefore, use of the Christensen and Anderson model is strictly suitablefor characterizing the response of asphalt binders from low to intermediate temperatures. To describe the temperature dependency of shift factors, both the WLF and theArrhenius function were used. At temperatures lower than a certain limit (designated by adefining temperature), an Arrhenius function, defined by the following equation, was usedto characterize the temperature dependency of asphalt: Ha  1 1  log a T =  − , (2.29) 2.303 R  T Td  33
41. 41. where, H a = activation energy for flow below Td , J/mol, R = ideal gas constant, 8.304 J/mol.°K, Td = defining temperature, °K or °C.At temperatures above Td , the WLF equation yielded reasonable values for shift factors.A strong correlation between Td and Tg was suggested, however, no explicit relationshipbetween the two was ever established.2.8.5 Gahvari’s Model Gahvari performed dynamic mechanical analysis on 21 asphalt-polymer blends. Adynamic shear rheometer was used to test original asphalt-polymer blends as well astheir RTFO residue. Models for storage and loss modulus were developed in order todiscuss the frequency dependence of response. The model for storage modulus is givenby:logG’ = logGg [1 − e − p (logω + l ) ] (2.30)where, G’(ω) = storage modulus, Gg = glassy modulus, p= proportionality factor, l = location parameter for the master curve = log 1/ωG’=1. 34
42. 42. Gahvari observed that the variation of the storage modulus between the twoasymptotic extremes followed an exponential pattern, which can be described byMitcherlich’s law of diminishing returns (1909). This law states that the rate of increasein value of certain functions is proportional to the difference between the maximumasymptotic and actual values of the function. The model proposed by Gahvari, forstorage modulus, adequately characterized the frequency dependence of the material formoduli below 108 Pa. Above this limiting value, this model tends to overestimate themodulus. The model proposed for characterizing the frequency dependence of loss modulus isa hyperbolic equation given by: logG" (w ) = (logG"max +d ) − (logω − logω d )2 + d 2 (2.31)where, G”(ω) = loss modulus Pa, ω = reduced frequency, rad/s, G”max = peak value of the loss modulus, Pa, d = half length of the transverse axis, Pa, and ωd = location parameter for the master curve, rad/s = ωG”= G”maxThis equation represents one arm of a rectangular hyperbola centered at (logωd,logG”max+d) on the logω - logG’’ coordinate system. At low frequencies, the hyperbolaapproaches an asymptote whose equation is given by: logG’’(ω)=(logω - logωd) + (logG’’max + d) (2.32) 35
43. 43. This equation represents the viscous asymptote of response, and is given by a line with aslope of unity on the same coordinate system. It was observed that the value of ωd variedwith polymer type. Higher ωd values were observed for binders modified with blockcopolymers as compared to those modified with SBR. It was also found that ωd increasedwith increasing polymer content. However, with constant polymer content, agingtreatment caused the value of ωd to shift backward. The parameter d, defined as a shape factor, is similar to the constant β in Dickinsonand Witt’s Model. With equal polymer concentration levels, the asphalt-polymer blendscontaining block copolymers exhibited considerably higher d values than those modifiedwith random copolymers. Short term aging of the binder resulted in a significant increasein the value of d. G’’max, the peak value of loss modulus, was found to be a characteristic of the baseasphalt. This parameter was not appreciably influenced by the addition of polymer oraging treatment. The value of G’’max was measured to be approximately 107.5 Pa. The model for frequency dependence of the loss modulus fit the experimental dataover the entire range of reduced frequencies. However, there was no experimental dataavailable to demonstrate the behavior of the model above ωd. The proposed model ishyperbolic and is symmetric to the line logω = logωd. The shape of the loss modulusmaster curve is not symmetrical in shape with respect to the peak point; therefore, theuse of this model is restricted to the specified range of moduli values less than or equal to107.5 Pa. The temperature dependency of the shift factors was found to follow the WLFequation with universal constants. 36
44. 44. 2.8.6 Stastna’s Model Stastna, et al. (1996) proposed a simple model of the complex modulus and phaseangle based on a generalization of the Maxwell model. Dynamic mechanical analysiswas performed on five modified and some 19 different unmodified asphalt binders. Theproposed equation for complex modulus is given by: 1 /( n − m )  m 2   ∏ [1 + (ωµ k ) ]    G *ω ) = iη 0ω  1 n  (2.33)  ∏ [1 + (ωλ ) 2 ]   1  k   π m n  δ (ω ) = + β  ∑ arctan(µ kω ) − ∑ arctan(λkω ) (2.34) 2  1 1 where, m < n, µk > 0, λk > 0, η0 > 0; µk and λk represent relaxation times; and η0 represents the zero-shear viscosity. Equations (2.33) and (2.34) were able to model the response of polymer modifiedasphalts with a limited number of parameters (between 10 to 15). Each parameter isbinder specific and must be determined through regression analysis and experimentaldata. When applied to a typical experimental data set, the model lacks statistical vitality,because the number of unknown parameters approaches the degrees of freedom in thedata (Marasteanu and Anderson, 1999). 37
45. 45. 2.8.7 Marasteanu and Anderson Model Marasteanu and Anderson (1999) modified the model developed by Christensen andAnderson (1992) in order to accomadate modified binders. The researchers applied theHavriliak and Negami model to the |G*|, resulting in the following equation: v − G * (ω ) = Gg [1 + (ω c / ω ) v ] w (2.35) 90 δ (ω ) = v (2.36) ω  1+   ω   cwhere, v = log2/R, and ωc = describes the slope of the phase angle curve.This model was applied to 38 plain and modified binders, and the degree of precision ofthe improved equation was found to be greater than the original model. All of the aforementioned models were developed based on experimental dynamicmechanical data from straight asphalt binders, with the exception of those presented byGahvari and Al-Qadi (1996), Stastna et al. (1996), and Marasteanu and Anderson (1999).The frequency dependence models are successful in describing the overall shape of themaster curves but they are either mathematically complex or have some aforementionedlimitations in the range of application. 38
46. 46. Chapter 3. Research Program The experimental plan, conducted in earlier research at Virginia Tech, consisted of the measurement of the complex moduli of 21 asphalt-polymer blends at frequencies between 0.06 to 188.5 rad/s and temperatures ranging from 5 to 75°C. The mixes were prepared using a conventional AC-20 paving grade asphalt binder and seven different elastomeric polymer modifiers. Each polymeric additive was blended with asphalt binder at three different concentration levels. The modifiers used were thermoplastic block copolymers and random copolymers, which are commonly used in industry and represent a wide range of chemical structures, and mechanical and physical properties. The study also investigated the effect of short-term aging on the rheological properties of the polymer-modified asphalt blends.3.1 Materials and Specimen Preparation All tested samples were prepared at the Structures and Materials Laboratory atVirginia Tech (Gahvari, 1995). The base asphalt was a grade AC-20 asphalt that wassupplied by Amocco Oil Company. Table 3-1 shows the conventional test results for theasphalt used. Seven different elastomeric polymers were used in this study: two styrene-butadiene-rubber (SBR) random copolymers, two styrene-butadiene-styrene (SBS) blockcopolymers, two styrene-butadiene/butylene-styrene (SEBS) linear block copolymers,and one (SB)n branched copolymer. Typical properties for these copolymers arepresented in Tables 3-2 and 3-3. The tables also indicate the designation adopted toidentify the copolymers during experimentation. The two SEBS linear block copolymers were supplied by the manufacturer in the formof a fine uniform powder, which is suitable for mixing with asphalt due to the high surfacearea of particles. 39
47. 47. Table 3-1. AC-20 Properties. Specimen Condition Unaged (RTFO)Specific Gravity 1.037 (N/A)Penetration at 25°C (0.01 mm) 66 40Absolute Viscosity at 60°C 2054 4232(poise)Kinematic Viscosity at 135°C 4437 (N/A)(cSt) Table 3-2. Typical properties of the random modifiers.Designation P CPhysical Form Emulsion EmulsionSolid Content 68 68Specific Gravity .95 .95pH 10 10Brookfield Viscosity, cps 1300 1300Styrene Butadiene Ratio 24/76 24/76 40
48. 48. Table 3-3. Typical properties of the thermoplastic block copolymer modifiers at 23oC. Designation S D G X N Structure Linear Linear Radial Linear SBS Linear SEBS SBS SEBS (SB)n Physical Form Porous Porous Porous Pellet Powder Powder Pellet Pellet Plasticizer Oil Content 0 29 0 0 0 (%w) Specific Gravity .94 .93 .91 .92 .94 BrookfieldViscosity at 25°C 4000 1000 1350 5370 20000 (cps)Tensile Strength, Pa 31700 19000 31050 24150 27600 (ASTM D 412)300% Modulus, Pa (ASTM D 412) 2760 1720 4830 6210 5520 Elongation , % (ASTM D 412) 880 1300 500 700 820Styrene/Butadiene Ratio 31/69 31/69 29/71 31/69 30/70The linear block copolymers (SBS) and the branched copolymer (SB)n were reducedusing a laboratory granulator, because the particle size was too large to assure propermixing. The grounded polymers were passed through a 1.19mm sieve to obtain a fineand uniform mix. 41
49. 49. Blending was performed using a Lightnin Labmaster laboratory mixer. All polymerswere blended with the asphalt binder at three different concentration levels. For therandom copolymer designated as C, the concentration levels were 2, 3, and 4% by weightof asphalt. All other polymers were blended at 3, 4, and 5%. Depending on the polymertype, the mixing temperature ranged from 163° to 177°C. With the mixer operating at alow speed, the binder was heated to the desired temperature. Once this temperature wasreached, the polymer was added slowly in order to avoid agglomeration of the polymericparticles. The main mixing cycle started at an increased speed after the addition ofpolymer, and continued for a one to 10 hr period, depending on the polymer type andcontent. The beaker was then transferred to an oven maintained at 163°C and allowed tostay for approximately one hr. If no obvious signs of phase separation between polymerand binder were observed, the blend was poured in several small containers. Thesecontainers were sealed, marked for identification, and stored at room temperature forfurther testing. Immediately after blend preparation, samples of each modified asphalt were aged inaccordance with the rolling thin film oven test (RTFOT) procedure, ASTM D 2872 (AnnualBook of Standards, 1991). The aged samples were then transferred to smallercontainers, marked for identification, sealed, and stored at room temperature. A four-character code was used to designate each polymer-asphalt combination. Thefirst character, A, refers to the type of asphalt, Amoco AC-20. The second characterdescribes the aging condition of the binder, U for unaged and R for RTFO residue. Thepolymer type and concentration percentage is given by the third and fourth characters,respectively. For example, a blend of unaged asphalt with 5% polymer N (radial SBn) isdesignated as ARN5.3.2 Data Collection and Analysis The binders were tested using a Bohlin stress-controlled dynamic shear rheometer(DSR) with parallel plate configuration. Measurement temperatures ranged from 5° to 42
50. 50. 75°C with increments of 10°C. The 8-mm plate was used for performing tests attemperatures of 5° to 35°C, and the 25-mm plate was used for tests at 35° to 75°C.Specimens were completely immersed in a temperature-controlled water bath with forcedcirculation in order to maintain the specified constant temperature during testing. The 25-mm-diameter binder specimens were prefabricated using a silicon rubber mold, and the8-mm-diameter specimens were poured directly between the two plates and trimmed tothe desired geometry. The linear viscoelastic range was determined for each binder-polymer blend in bothaged and unaged conditions by performing stress sweeps over the entire range oftemperatures and specified frequencies. Limiting strains were determined from the stresssweeps and then reduced to a uniform range for all binders, which were later used astarget strains in performing frequency sweeps. The target strains for 5, 15, 25, 35, and45°C were 0.8, 1, 2, 3, and 6.5%, respectively. For temperatures above 55 °C, the targetstrain was was found to be 9%. These strains are well within the linear range of responseas established by the stress sweeps, and are below the values stated by AASHTO TP5(AASHTO Provisional Standards, 1994) for straight binders. Frequency sweeps werethen performed on all samples over the entire range of temperatures. Thirty-fourfrequencies ranging from 0.063 to 188.5 rad/s were used. Two replicate specimens weretested for each binder.3.3 Comparison of Recent and Previous Data Analysis The experimental data for dynamic moduli functions were obtained from the originalfrequency sweeps. The principle of time-temperature superposition was found to beapplicable. For each polymer asphalt combination, isothermal graphs of complex,storage, and loss moduli data were plotted against frequency on a log-log scale. Generally it is accepted to use either the loss or storage modulus in determining theamount of translation along the frequency axis in the construction of master curves.Figures 3-1 and 3-2 show the isothermal plots for storage and loss moduli for the sample 43
51. 51. designated as ARG3. The storage modulus measurements tend to yield erroneousreadings at high temperatures (very low frequencies on the translated frequency axis).This is expected, because at very high temperatures, the complex shear modulus isalmost entirely composed of the loss modulus. The shapes of these curves are skewedand are not suitable for use in developing a smooth master curve over the entire range offrequencies. For this research, master curves for the dynamic moduli were preparedusing the time-temperature superposition principle based on the loss modulusmeasurements. Two sets of dynamic moduli master curves were constructed for eachpolymer-asphalt blend using the replicate specimen data. Figures 3-3 and 3-4 show thedynamic loss and storage moduli, as well as the loss tangent master curve for ARG3. The isothermal curve corresponding to 25°C was used as the reference temperaturefor construction of the master curves. All other segments were translated along thefrequency axis to obtain a smooth unique curve. The translation was accomplished usinga spreadsheet and visual inspection of corresponding graphs to find the best possible fit.The same shift factors derived from the loss moduli apply to the remaining viscoelasticfunctions. Dynamic loss modulus master curves, shift factor, and isothermal graphs arepresented in Appendix A. 44
52. 52. 1.00E+08 5°C 15°C 25°C 35°CStorage Modulus (Pa) 45°C 1.00E+05 55°C 65°C 75°C 1.00E+02 1.00E-01 1.00E-02 1.00E-01 1.00E+00 1.00E+01 1.00E+02 1.00E+03 Reduced Frequency (rad/s) Figure 3-1. Dynamic storage modulus versus frequency at eight test temperatures for ARG3. 45
53. 53. 1.00E+08 5°C 15°C 25°C 35°C 1.00E+06 45°CLoss Modulus (Pa) 55°C 65°C 75°C 1.00E+04 1.00E+02 1.00E+00 1.00E-03 1.00E-01 1.00E+01 1.00E+03 Reduced Frequency (rad/s) Figure 3-2. Dynamic loss modulus versus frequency at eight test temperatures for ARG3. 46
54. 54. 1.00E+09 1.00E+07Modulus (Pa) 1.00E+05 1.00E+03 1.00E+01 Storage modulus Loss modulus 1.00E-01 1.00E-06 1.00E-03 1.00E+00 1.00E+03 1.00E+06 Reduced Frequency (rad/s)Figure 3-3. Dynamic storage modulus and loss modulus master curves for ARG3 (reference temperature 25°C). 47
55. 55. 1.00E+03Loss Tangent (Pa) 1.00E+01 1.00E-01 1.00E -06 1.00E-03 1.00E +00 1.00E +03 1.00E+06 R educed Frequency (rad/s) Figure 3-4. Loss tangent master curve for ARG3 (reference temperature 25°C). 48
56. 56. Chapter 4. Model Development for Frequency Dependency of Loss Moduli4.1 Background During the primary analysis of the experimental data, several Master Curves wereconstructed for the purpose of developing a model to predict the frequency response ofthe loss modulus. It is previously noted that the models described in Chapter 2 forpredicting the frequency response of straight asphalt binders are not applicable topolymer-modified binders (Gahvari, 1995). In most cases, considerable discrepancieswere observed between the experimental results and data generated by the mathematicalmodels for straight binders. Gahvari (1995) attempted to fit the complex modulus data to a number of sigmodalfunctions. The Weibull distribution function, logistic equation, Gompertz growth model,and Mitcherlich’s equation were among the different models used for this purpose. Noneof these models were successful in predicting the response of the complex modulus.Similar results were encountered when applying the aforementioned models to thedynamic loss moduli data. Figure 4-1 compares the experimental data for loss moduliwith data generated from the logistic model. The logistic model provides a relatively goodfit for loss moduli values above 105 Pa. Below this value, a moderately good fit isobtained until 102 Pa is reached, at which point the model overestimates the experimentaldata. However, the Gompertz growth model was successfully used to characterize theloss moduli data over the entire range of reduced frequencies. 49